General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.65 - 7.7 g/cm³ Show Material materials with Density of 7.65 - 7.7 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 196 - 231.66 GPa Show Material materials with Elastic modulus of 196 - 231.66 GPa |

95.0 °C | 227.53 GPa Show Material materials with Elastic modulus of 227.53 GPa | |

100.0 °C | 215 GPa Show Material materials with Elastic modulus of 215 GPa | |

150.0 °C | 223.39 GPa Show Material materials with Elastic modulus of 223.39 GPa | |

200.0 °C | 210 GPa Show Material materials with Elastic modulus of 210 GPa | |

205.0 °C | 218.56 GPa Show Material materials with Elastic modulus of 218.56 GPa | |

260.0 °C | 213.74 GPa Show Material materials with Elastic modulus of 213.74 GPa | |

300.0 °C | 205 GPa Show Material materials with Elastic modulus of 205 GPa | |

315.0 °C | 209.6 GPa Show Material materials with Elastic modulus of 209.6 GPa | |

370.0 °C | 204.09 GPa Show Material materials with Elastic modulus of 204.09 GPa | |

400.0 °C | 195 GPa Show Material materials with Elastic modulus of 195 GPa | |

425.0 °C | 198.57 GPa Show Material materials with Elastic modulus of 198.57 GPa | |

485.0 °C | 193.05 GPa Show Material materials with Elastic modulus of 193.05 GPa | |

540.0 °C | 187.54 GPa Show Material materials with Elastic modulus of 187.54 GPa | |

595.0 °C | 180.64 GPa Show Material materials with Elastic modulus of 180.64 GPa | |

650.0 °C | 173.06 GPa Show Material materials with Elastic modulus of 173.06 GPa | |

705.0 °C | 162.72 GPa Show Material materials with Elastic modulus of 162.72 GPa | |

760.0 °C | 151.69 GPa Show Material materials with Elastic modulus of 151.69 GPa | |

815.0 °C | 144.79 GPa Show Material materials with Elastic modulus of 144.79 GPa | |

Hardness, Brinell | 20.0 °C | 200 [-] Show Material materials with Hardness, Brinell of 200 [-] |

Poisson's ratio | 20.0 °C | 0.24 [-] Show Material materials with Poisson's ratio of 0.24 [-] |

95.0 °C | 0.27 [-] Show Material materials with Poisson's ratio of 0.27 [-] | |

150.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

205.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

260.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

315.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

370.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

425.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

485.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

540.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

595.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

650.0 °C | 0.34 [-] Show Material materials with Poisson's ratio of 0.34 [-] | |

705.0 °C | 0.34 [-] Show Material materials with Poisson's ratio of 0.34 [-] | |

760.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

815.0 °C | 0.35 [-] Show Material materials with Poisson's ratio of 0.35 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 93.08 GPa Show Material materials with Shear modulus of 93.08 GPa |

95.0 °C | 89.63 GPa Show Material materials with Shear modulus of 89.63 GPa | |

150.0 °C | 87.56 GPa Show Material materials with Shear modulus of 87.56 GPa | |

205.0 °C | 84.81 GPa Show Material materials with Shear modulus of 84.81 GPa | |

260.0 °C | 82.74 GPa Show Material materials with Shear modulus of 82.74 GPa | |

315.0 °C | 81.36 GPa Show Material materials with Shear modulus of 81.36 GPa | |

370.0 °C | 79.29 GPa Show Material materials with Shear modulus of 79.29 GPa | |

425.0 °C | 77.22 GPa Show Material materials with Shear modulus of 77.22 GPa | |

485.0 °C | 74.46 GPa Show Material materials with Shear modulus of 74.46 GPa | |

540.0 °C | 71.71 GPa Show Material materials with Shear modulus of 71.71 GPa | |

595.0 °C | 68.95 GPa Show Material materials with Shear modulus of 68.95 GPa | |

650.0 °C | 64.81 GPa Show Material materials with Shear modulus of 64.81 GPa | |

705.0 °C | 60.67 GPa Show Material materials with Shear modulus of 60.67 GPa | |

760.0 °C | 57.23 GPa Show Material materials with Shear modulus of 57.23 GPa | |

815.0 °C | 53.78 GPa Show Material materials with Shear modulus of 53.78 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 400 - 630 MPa Show Material materials with Tensile strength of 400 - 630 MPa |

Yield strength Rp0.2 | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp0.2 of 240 MPa |

100.0 °C | 220 MPa Show Material materials with Yield strength Rp0.2 of 220 MPa | |

150.0 °C | 215 MPa Show Material materials with Yield strength Rp0.2 of 215 MPa | |

200.0 °C | 210 MPa Show Material materials with Yield strength Rp0.2 of 210 MPa | |

250.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2 of 205 MPa | |

300.0 °C | 200 MPa Show Material materials with Yield strength Rp0.2 of 200 MPa | |

350.0 °C | 195 MPa Show Material materials with Yield strength Rp0.2 of 195 MPa | |

400.0 °C | 190 MPa Show Material materials with Yield strength Rp0.2 of 190 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 9.2E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.2E-6 1/K | |

20.0 °C | 9.9E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.9E-6 1/K | ||

100.0 °C | 1E-5 - 1.03E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 - 1.03E-5 1/K | ||

200.0 °C | 1E-5 - 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 - 1.08E-5 1/K | ||

300.0 °C | 1.05E-5 - 1.12E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.12E-5 1/K | ||

400.0 °C | 1.05E-5 - 1.16E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.16E-5 1/K | ||

500.0 °C | 1.1E-5 - 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.1E-5 - 1.19E-5 1/K | ||

600.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

700.0 °C | 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 1/K | ||

800.0 °C | 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 1/K | ||

900.0 °C | 1.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.34E-5 1/K | ||

1000.0 °C | 1.39E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.39E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1425 - 1530 °C Show Material materials with Melting point of 1425 - 1530 °C | Typical for Ferritic Stainless Steel | |

Specific heat capacity | 20.0 °C | 450 - 460 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 460 J/(kg·K) | |

100.0 °C | 482 J/(kg·K) Show Material materials with Specific heat capacity of 482 J/(kg·K) | ||

200.0 °C | 506 J/(kg·K) Show Material materials with Specific heat capacity of 506 J/(kg·K) | ||

300.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

400.0 °C | 547 J/(kg·K) Show Material materials with Specific heat capacity of 547 J/(kg·K) | ||

500.0 °C | 576 J/(kg·K) Show Material materials with Specific heat capacity of 576 J/(kg·K) | ||

600.0 °C | 616 J/(kg·K) Show Material materials with Specific heat capacity of 616 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 19.6 - 25 W/(m·K) Show Material materials with Thermal conductivity of 19.6 - 25 W/(m·K) | |

Thermal diffusivity | 20.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 6.17E-7 Ω·m Show Material materials with Electrical resistivity of 6.17E-7 Ω·m |

Chemical properties

Property | Value |
---|---|

Carbon | 0.08 % Show Material materials with Carbon of 0.08 % |

Chromium | 16 - 18 % Show Material materials with Chromium of 16 - 18 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.03 % Show Material materials with Sulfur of 0.03 % |